Copyright and moral rights for the publications made accessible in the public portal are retained by the authors and/or other copyright
owners and it is a condition of accessing publications that users recognise and abide by the legal requirements associated with these rights.
Users may download and print one copy of any publication from the public portal for the purpose of private study or research.
You may not further distribute the material or use it for any profit-making activity or commercial gain
You may freely distribute the URL identifying the publication in the public portal
If you believe that this document breaches copyright please contact us providing details, and we will remove access to the work immediately
and investigate your claim.
Downloaded from orbit.dtu.dk on: Jun 24, 2021
Influence of surface pretreatment in resistance spot welding of aluminum AA1050
Al Naimi, Ihsan K.; Al Saadi, Moneer H.; Daws, Kasim M.; Bay, Niels Oluf
Production & Manufacturing Research
Link to article, DOI:
Publisher's PDF, also known as Version of record
Link back to DTU Orbit
Al Naimi, I. K., Al Saadi, M. H., Daws, K. M., & Bay, N. O. (2015). Influence of surface pretreatment in resistance
spot welding of aluminum AA1050. Production & Manufacturing Research, 3(1), 185-200.
Full Terms & Conditions of access and use can be found at
Download by: [DTU Library] Date: 27 May 2016, At: 03:39
Production & Manufacturing Research
An Open Access Journal
ISSN: (Print) 2169-3277 (Online) Journal homepage: http://www.tandfonline.com/loi/tpmr20
Influence of surface pretreatment in resistance
spot welding of aluminum AA1050
Ihsan K. Al Naimi, Moneer H. Al Saadi, Kasim M. Daws & Niels Bay
To cite this article: Ihsan K. Al Naimi, Moneer H. Al Saadi, Kasim M. Daws & Niels Bay (2015)
Influence of surface pretreatment in resistance spot welding of aluminum AA1050, Production
& Manufacturing Research, 3:1, 185-200, DOI: 10.1080/21693277.2015.1030795
To link to this article: http://dx.doi.org/10.1080/21693277.2015.1030795
© 2015 The Author(s). Published by Taylor &
Published online: 02 Apr 2015.
Submit your article to this journal
Article views: 673
View related articles
View Crossmark data
Influence of surface pretreatment in resistance spot welding of
Ihsan K. Al Naimia*, Moneer H. Al Saadib, Kasim M. Dawsa and Niels Bayc
aMechanical Department, College of Engineering, Baghdad University, Baghdad, Iraq; bWelding
Department, University of Kerbala, Baghdad, Iraq; cDepartment of Mechanical Engineering,
Technical University of Denmark, Lyngby, Denmark
(Received 23 November 2013; accepted 15 March 2015)
Resistance spot welding (RSW) of aluminum alloys implies a major problem of
inconsistent quality from weld to weld due to problems of varying thickness of the
oxide layer. The high resistivity of oxide layer causes strong heat development,
which has significant influence on electrode life and weld quality. An experimental
study of the influence of pretreatment on weld quality in RSW of AA1050 sheets
with three thicknesses, comparing welding of as-received sheet with pretreated sheet
by either pickling in NaOH or glass-blasting were investigated. Different weld set-
tings were applied with low-, medium-, and high-energy inputs. The as-received
sheet showed higher electrical contact resistance because of thicker oxide layer.
Lower values were noticed with pickled surfaces, whereas the lowest electrical
contact resistance was obtained when glass blasting, resulting in the roughest surface
topography, which facilitated breakdown the oxide layer. Highest strength and
smaller scatter in strength were obtained by pickling in NaOH.
Keywords: resistance spot welding; contact resistance; oxide film; surface
The increasing demands for energy savings have implied special focus in automotive
industry on lighter vehicles production, among other solutions by introducing skin pan-
els of aluminum instead of steel. Weight savings up to 46% are reported (Wheeler,
Sheasby, & Kewley, 1987), and furthermore resistance to corrosion is improved.
Resistance spot welding (RSW) is the most dominant process in sheet metal joining,
particularly in automotive industry due to low cost, high productivity, flexibility, easy
automation and maintenance, and minimum requirements for skilled labor (Brown,
Newton, & Boomer, 1995; Cho, Li, & Hu, 2006; Spinella, Brockenbrough, & Fridy,
2005). The process is also widely applied in other industries of sheet product manufac-
turing, e.g. other transportation industries and in production of kitchen utensils.
It should, however, be emphasized that RSW of aluminum is more problematic than
steel due to higher electrical and thermal conductivity, higher coefficient of expansion,
lower melting temperature, and an oxide layer, which has high electrical resistance and
high melting temperature (2050 °C). The latter together with the fact that the effective
contact resistance grows considerably as the oxide film grows implies large scatter in
*Corresponding author. Email: firstname.lastname@example.org
© 2015 The Author(s). Published by Taylor & Francis.
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecom
mons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided the original
work is properly cited.
Production & Manufacturing Research: An Open Access Journal, 2015
Vol. 3, No. 1, 185–200, http://dx.doi.org/10.1080/21693277.2015.1030795
quality of RSW aluminum sheets, which therefore require close production control
(Boomer, Hunter, & Castle, 2003; Kim, Park, Hwang, & Kang, 2009; Mathers, 2002).
The high thermal and electrical conductivity of aluminum require 2–3 times higher
current and shorter weld time, typically 25% of that used to spot weld steel. Accurate
control and synchronization of current and electrode force is required due to the narrow
weld temperature range (Resistance Welding Manual, 2003). The problems are espe-
cially pronounced when welding unalloyed aluminum AA 1XXX.
Aluminum is highly reactive to oxygen, and after removal of the oxide layer by
mechanical or chemical means, a new oxide layer will immediately form on its surface
in normal atmosphere. The layer is beneficial as it protects the base metal from corro-
sion, but creates problems in connection with resistance welding, where it causes severe
electrode degradation and scatter in weld quality due to (Han, Thornton, Boomer, &
Shergold, 2010; Patrick, Auhl, & Sun, 1984; Sun, 1982). Spot welding in aluminum
AA1050 is less stable than in alloyed aluminum, and the electrodes will stick to the
sheet after 50 welds because of the oxide film problems (Pedersen, 2010). Contributions
to the contact resistance comes from the oxide layer as well as the contaminant film,
which may include dirt, lubricant, chemicals, and water vapor (Rashid, 2011; Sun,
2003). Even though maintenance of uniform surface conditions is taken carefully into
consideration, the electrical contact resistance will vary from weld to weld implying
inconsistent weld quality.
Contact resistance was experimentally investigated by Song, Zhang, and Bay (2005)
using a Gleeble system. They showed that interface normal pressure had significant but
decreasing influence on the contact resistance with increasing normal pressure, whereas
the influence of temperature was less pronounced as pressure increased. Surface rough-
ness together with elastic–plastic properties of the materials also influences the electrical
contact resistance (Dzekster & Ismailov, 1990; Zheng, Shan, Hu, & Luo, 2006). Crinon
and Evans (1998) showed that the effect of the oxide film is greatest for specimens with
the smoothest surface.
Expulsion during RSW may either occur at the faying surfaces or the elec-